untitledEnhanced Young’s Modulus of AlSi Alloys and Reinforced
Matrices
by Co-continuous Structures
Institute of Materials Science and Technology, Vienna University of
Technology
Karlsplatz 13/E308, A-1040 Vienna, Austria
ABSTRACT: In the present work, the elastic behavior of different
hypoeutectic and hypereutectic AlSi alloys and different Al2O3
short fiber and SiC particle reinforced materials (SFRM and PRM,
respectively) is studied. The effective Young’s modulus (E) of
materials was experimentally measured and compared with the
different theoretical predictions of HashinStrikman, Tuchiniskii,
shear lag, and the rule of mixtures (ROM). The unreinforced alloys
present an interconnected lamellar Si structure after fast
solidification, which increases the Young’s modulus up to that of
the Tuchiniskii prediction for interpenetrating skeletal
structures. On the other hand, alloys presenting isolated and
coarse Si particles (after spheroidization treat- ment at 540C) are
well described by the lower bound of the ROMs. Similarly, the
interconnected SiSiC structure observed in 10 and 70 vol% SiC
reinforced AlSi7Mg and AlSi7 matrices in the as cast condition is
responsible for the higher stiffness of the composite, if compared
with that of Al99.5 or spheroidized AlSi7 matrices. An analogous
behavior is observed in the SFRMs in the as cast condition, where
the Si lamellae bridge the Al2O3 fibers, increasing the Young’s
modulus of the composites, if compared with the conditions of
spheroidized Si. Furthermore, the primary Si particles produce an
improvement in the Young’s modulus by connecting several fibers in
the case of a short fiber-reinforced hypereutectic AlSi18
matrix.
KEY WORDS: AlSi alloys, metal matrix composites (MMCs),
Interpenetrating Si network, Young’s modulus, theoretical
estimations.
INTRODUCTION
T HE EXCELLENT CASTABILITY and mechanical properties of AlSi alloys
make them popular foundry alloys. The morphology of these alloys
depends strongly on the Si
content as well as on the casting process. As cast hypoeutectic
alloys contain dendritic primary a-phase with an interpenetrating
eutectic structure in between and between the
*Author to whom correspondence should be addressed. E-mail:
[email protected] **Current address: FADA-CATEC, C/Wilbur y
Orville Wright, 17-19-21, 41309 La Rinconada Seville, Spain.
Journal of COMPOSITE MATERIALS, Vol. 44, No. 6/2010 739
0021-9983/10/06 073917 $10.00/0 DOI: 10.1177/0021998309347649 The
Author(s), 2010. Reprints and permissions:
http://www.sagepub.co.uk/journalsPermissions.nav
secondary dendrite arms. The Si solidifies as an interpenetrating
network [1,2] of thin (12 mm) lamellae within the inter-dendritic
spaces. Solution treatment of alloys contain- ing more than 2wt% Si
produces the spheroidization of the eutectically solidified Si,
improving the ductility of the alloys.
Aluminum Matrix Composites are considered for use in highly
demanding automotive engines because of enhanced specific strength
and stiffness at elevated temperatures provided by the ceramic
reinforcement and some toughness by the Al-alloys [35]. Continuous
structures of rigid phases enhance the stiffness of composites, if
compared with discontinuously reinforced structures [68]. Stiffness
is the main design criterion for structural components; increasing
specific stiffness by interpenetrating structures allows a
reduction in weight. Several researchers have conducted work in
order to investigate the effect of the reinforcement connectivity
in co-continuous structures: Peng et al. [9] reports on
manufacturing and Young’s modulus (E) estimation of infiltrated
reticulated alumina preforms. For a given ceramic volume fraction,
these composites possess higher Young’s modulus than that of metal
matrix composites (MMCs) with homogeneous reinforcement
distribution [9,10]. In [11] a complete investigation of the
experimental and modeled Young’s modulus of several
Al-interpenetrating composites is presented. Particularly, it is
observed for the case of an AlSi12 alloy reinforced by 540% of an
Al2O3 continuous preform a good correlation with Tuchinskii model
[12] for interpenetrating structures (see section ‘Tuchinskii
Model’). Unfortunately, the effect of Si connectivity was not spe-
cifically studied. In [13] an interesting approach for predicting
the elastic properties of interpenetrating multiphase composites is
presented.
The objective of the present work is to investigate the effect of
connectivity on the effective Young’s modulus of several AlSi
alloys in the range 018wt% Si, as well as in several particle and
short fiber-reinforced AlSi matrices. The experimental results are
compared with numerous analytical models based on different
microstructural architec- tures. The role of the Si morphology is
analyzed and related to the elastic behavior of these
materials.
EXPERIMENTAL METHODS
Material Preparation
Three different types of materials were used in this work:
AlSi-alloys; Al2O3 short fiber- reinforced materials (SFRMs), and
SiC particle reinforced materials (PRMs). The AlSi-alloys were
produced using a squeeze casting process by ARCLeichtmetall
Kompetenzzentrum Ranshofen (LKR), Austria. The Si content of the
matrices was adjusted to AlSi1, a hypoeutectic AlSi7 alloy, a near
eutectic AlSi12 and a hypereutectic AlSi18 alloy. 20 vol% Al2O3
preforms (produced by Thermal Ceramics de France S.A.) were
infiltrated with the different matrices to produce four different
SFRMs, hereafter designated as AlSiX/Al2O3/20s. Two AlSi7Mg and
Al99.5 matrices were reinforced with 70 vol% SiC particles using a
gas pressure infiltration method (by Electrovac GmbH,
Kloesterneuburg, Austria) to produce two PRMs Al99.5/SiC/70p and
AlSi7Mg/SiC/70p, respectively. The particle preforms were prepared
from three modal powder sizes of aver- age 80 mm (55 vol%), 20 and
5 mm (some details on fabrication process are given in [14]). The
chemical composition of the alloys and matrices (provided by
materials suppliers) is depicted in Table 1. A 10 vol% SiC particle
reinforced AlSi7 alloy (AlSi7/SiC/10p) was
740 F. LASAGNI AND H. P. DEGISCHER
produced by stir casting at the Instituto Universitario de
Materiales de Alicante of the Alicante University. For all
materials, the reinforcement volume fraction was estimated by
density measurements or metallographic determinations.
Samples of the AlSi-alloys, the SFRMs, and AlSi7/SiC/10p were
solution treated (ST) at 540C for 4 h (or 80min in AlSi7/SiC/10p)
using a Linn High Therm furnace 70.26 in order to spheroidize the
eutectic Si-phase, and consecutively slowly cooled in air. The
AlSi7Mg/SiC/70p composite was tested in the overaged condition
(180C/ >10 h) to avoid the age hardening effect of Mg2Si
precipitates.
Imaging of Percolating Networks
Small samples (4 4 10mm3) of the unreinforced AlSi alloys in the as
cast condition and composite materials in the as cast condition and
after ST treatment were leached using 17wt% HCl (during 48 h) to
remove the Al-phase. A Si porous structure could be con- served
from the AlSi7, AlSi12, and AlSi18 alloys in the as cast condition,
while the ST samples disintegrated during chemical etching. A
self-supporting SiAl2O3 (SFRMs) and SiSiC (PRMs) structure was
extracted from the SFRMs with the as-cast alloy matrices and the
PRMs, as well as from the SFRMs with the matrices in the ST
condition. The extracted 3D networks were investigated using a FEI
strata DB 235 electron microscope.
Young’s Modulus Measurement
The Young’s modulus E of the unreinforced AlSi alloys and composite
materials was measured by means of a TA Instruments DMA 2980TM
dynamic mechanical analyzer using samples of 2 4 55mm3 size. Here,
the sample’s natural frequency of vibration was used to obtain the
Young’s modulus. The specimen displacement is monitored by a linear
variable differential transformer (LVDT) and the measured lag
between the drive signal and the LVDT is the phase angle. The phase
angle and drive signal are used to calculate the elastic modulus E0
and damping capacity E00 of the specimen [15]. In the case of the
short fiber-reinforced composites, the samples were cut so that the
4 55mm2 area was oriented parallel to the plane of random fiber
orientation. The Young’s modulus of the specimens was measured as a
function of temperature using a heating rate of 3K/min from room
temperature (RT) to 300C. At higher temperatures (>350C), the
energy loss component increases considerably due to plastic
deformation in the sample, giving erro- neous values of Young’s
modulus. The specimens were clamped and then subjected to a uniform
sinusoidal displacement of constant maximum amplitude of 40 mm. The
oscilla- tion frequency was fixed at 1Hz. Two samples or more for
each material were tested in
Table 1. Composition of the studied alloys and composites
(Al-balance).
Matrix Si (wt%) Mg (wt%) Fe (wt%) MMC
Al99.5 <0.3 <0.01 <0.4 Al99.5/SiC/70p AlSi1 1.11 <0.01
0.09 AlSi1.1/Al2O3/20s AlSi7 7.04 <0.01 0.07 AlSi7/Al2O3/20s
AlSi7/SiC/10p AlSi7Mg 6.57.5 0.30.45 0.18 AlSi7Mg/SiC/70p AlSi12
11.87 <0.01 0.08 AlSi12/Al2O3/20s AlSi18 17.86 <0.01 0.16
AlSi18/Al2O3/20s
Enhanced Young’s Modulus of AlSi Alloys and Reinforced Matrices
741
order to check the reproducibility of results, showing identical
results for each material in both AC and ST conditions.
In the case of Al99.5/SiC/70p and AlSi7Mg/SiC/70p composites, the
Young’s modulus has been determined by means of Elastotron 2000TM
at the Institute of Physics at the University of Vienna (by
Puchegger et al. [16]). This is achieved by free vibrating long
thin specimens of rectangular cross section (5 4.8 60mm3) supported
by carbon fibers [17]. The specimen hangs between graphite heating
elements in a vacuum chamber. The exper- imentally measured set of
resonant frequencies is precisely obtained by finding the roots of
the derivative response signal of the receiver and then compared
with predictions from theory based on Timoshenko’s equation. The
accuracy of this method is around 12%.
THEORETICAL ESTIMATIONS OF THE YOUNG’S MODULUS
OF TWO-PHASE COMPOSITES
The modeling of Young’s modulus of composite materials has been
estimated by means of several theoretical estimations, which depend
on the morphological arrangement of materials components. The
models were applied following the subsequent considerations: For
the case of the AlSi alloys the reinforcement phase was Si and the
matrix phase was Al. For the SFRMs, the reinforcement phase was the
Al2O3 fibers, and the matrix phase was the composite alloy (AlSi1,
AlSi7, AlSi12, and AlSi18) in the corresponding thermal condition
(AC or ST). In case of the PRMs, the reinforcement phase was SiC
and the composite alloy for the matrix (Al99.5, AlSi7, AlSi7Mg)
also in the corresponding thermal condition (AC or ST).
The volume fraction of the Si phase in AlSi alloys is calculated by
subtracting the maximum dissolved Si fraction at the eutectic
temperature (1.7wt%) from the nominal Si content. For the case of
the short fiber composites and 10 vol% composites, the Young’s
modulus was calculated using the experimental data of the
unreinforced matrices pre- sented in this work. Tables 2 and 3
summarize the input data for the different models (physical
constants and volume fraction of the different phases,
respectively).
Rule of Mixtures
For the purpose of comparison, the well-known rule of mixtures
(ROM) was used in this work for estimating the Young’s moduli of
the composites as if they were composed of two slabs bonded
together [18]. In case of normal stress being applied parallel to
the slab direction (equally strained phases), a weighted mean
between the moduli of the two components is obtained (ROM Voigt
model [18]):
EC ¼ EmVm þ ErVr, ð1Þ
where E and V are the Young’s modulus and the volume fraction of
the material compo- nents, and the subscripts m and r represent the
matrix and reinforcing phases, respectively. The prediction of the
transverse stiffness (equally stressed phases) gives the lower
bound which is often described as the ROM Reuss model [18]:
EC ¼ Vr
Er þ Vm
HashinShtrikman
The HashinShtrikman (HS) bounds [19] refer to isolated spherical
inclusions coated by a second phase. For this estimation no
inclusioninclusion interaction among neigh- boring inclusions is
considered. The upper HS bound is then analogous to the case in
which the softer phase is the inclusion material, while the lower
bound is equivalent to the case in which the stiffer phase is the
inclusion material. The HS lower bound can be calculated as
[10]:
EC ¼ Em½EmVm þ ErðVr þ 1Þ
ErVm þ EmðVr þ 1Þ : ð3Þ
Tuchinskii Model
This section was originally written by Moon et al. [11]. The
Tuchinskii model [12] considers a two-phase interpenetrating
skeletal structure, where a cube of height ‘H’ is composed of a
skeletal structure of phase 1, the cavity of which is filled with
phase 2 of a characteristic dimension h [11]. A repeating array of
unit cubes thus forms an interpenetrating skeletal structure for
both phases. The ratio of the lengths, c¼ h/H,
Table 3. Microstructural parameters for modeling of the Young’s
modulus.
Material Matrix/volume
fraction (%) Reinforcement/volume
fraction (%)
AlSi1 Al/100 Si/0 AlSi7 Al/92 Si/6.2 AlSi12 Al/82.3 Si/11.9 AlSi18
Al/79.7 Si/18.5 AlSiX/Al2O3/20s AlSiX/80 Al2O3/20b
AlSi7Mg/SiC/10p AlSi7Mg/90 10 Al99.5/SiC/70p Al99.5/30 70
AlSi7Mg/SiC/70p AlSi7Mg/30 70
Al2O3 short fibersa: r0¼ 2 mm, L¼ 68 mm, aspect ratio s¼ 34
aFrom microstructural quantification only for shear-lag estimation;
bin case of shear-lag estimation the effec- tive volume fraction of
short fibers was estimated by using correction factor of 2/5
(Effective vol. fraction¼8%¼ 20%2/5) [24].
Table 2. Physical constants for the modeling of Young’s moduli of
alloys and composites.
Component Young’s modulus (GPa) Poisson ratio
Al 69 [26] 0.33 [26] AlSi7Mg 74 [14] 0.33 [14] Si 162 [26] 0.22
[26] SiC 450 [26] 0.22 [26] Al2O3 370 [27] 0.22 [27] AlSi7a 74
(AC)/72 (ST) 0.33 AlSi12a 77 (AC)/75 (ST) 0.33 AlSi18a 84 (AC)/82.5
(ST) 0.33
aObtained experimentally in this work.
Enhanced Young’s Modulus of AlSi Alloys and Reinforced Matrices
743
can be related to the volume fraction of each phase, Vm+Vr¼ 1, by
the following
relationship:
Vm ¼ ð3 2cÞc2: ð4Þ
The effective composite Young’s modulus is calculated in two steps.
First, a unit cell is
sectioned, either parallel or perpendicular to the loading
direction, into three volume
elements, each having their own effective Young’s modulus, as
calculated using either
the iso-stress or iso-strain ROM models. Secondly, the volume
elements are ‘reassembled’
and the effective composite Young’s modulus of the unit cube is
then calculated by using
the ROM with the effective Young’s moduli of each layer. The
Tuchinskii upper bound is
calculated by initially sectioning perpendicular to the loading
direction and using the
ROM Voigt estimation in the final step, while the lower bound is
calculated by initially
sectioning parallel to the loading direction and using the ROM
Reuss equation in the final
step. The Tuchinskii upper (+) and lower () bounds are given by the
following
equations:
ð1 c2Þ þ ðEm=ErÞc2 þ
c
1 , ð5Þ
ECðÞ ¼ Er ð1 cÞ2 þ ðEm=ErÞc 2 þ
2ðEm=ErÞcð1 cÞ
Shear Lag
The most widely used model describing the effect of loading for
aligned short fiber
composites is the so-called shear-lag model, originally proposed by
Cox [20] and after-
wards developed by others [2123]. This model is based on the
transfer of tensile stress
from the matrix to the fibers by means of interfacial shear
stresses. The basis of these
calculations is well described in [18], where a comprehensive
mathematical treatment is
given. The external loading is applied parallel to the fiber axis.
The model is based on
considering the radial variation of shear stress in the matrix and
at the interface. In this
way, the axial Young’s modulus of the composite E3C can be
expressed as:
E3C ¼ VrEr 1 tan hðnsÞ
ns
n ¼ 2Em
1=2 , ð8Þ
and s is the fiber aspect ratio L/r0, L and r0 are the fibers’
length and radius, respectively,
and vm is the Poisson’s ratio of the matrix. The present model is
only used in this work for predicting the Young’s Modulus of
the
short fiber materials. Since the SFRMs present a random planar
distribution of the fibers
and the present model is based of simple aligned fiber to test
direction, the effective volume
fraction of the reinforcing phase must be corrected. Therefore, a
correction factor of 2/5
was applied in order to estimate the effective volume fraction of
fibers as proposed by
Dlouhy et al. [24]. Finally, the corrected volume fraction is
presented in Table 3.
744 F. LASAGNI AND H. P. DEGISCHER
MORPHOLOGICAL ANALYSIS
The 2D metallographies of the unreinforced AlSi7, AlSi12, and
AlSi18 alloys in the as
cast condition and of the AlSi12 after ST condition, are depicted
in Figure 1(a)(d). Both the AlSi7 and AlSi12 alloys behave
hypoeutectically, showing the primary a-phase enclosed by the
eutectic AlSi phase, and amounting to 75 and 25 vol%,
respectively
(these values were obtained after analyzing several low
magnification metallographies,
while only the eutectic structure is observed in the figures). The
AlSi12 alloys shows a
few primary Si particles of <0.1 vol% owing to the
nonequilibrium cooling conditions
experienced by the squeeze casting process. The interconnected Si
lamellae present a large
surface/volume ratio in 3D for all investigated as cast alloys
[25]. On the other hand, the
lamellar structure disintegrates and coarsens into rounded Si
particles [2] after heating at
540C for 4 h (ST condition). A continuous Si network is observed
after leaching of the Al-
phase in all the AlSi alloys in the as cast condition (e.g., AlSi7;
Figure 1(e)). The AlSi18
alloy presents mostly a eutectic composition and relatively large
primary Si particles of
around 5 vol%. Although this last alloy represents a hypereutectic
composition, less than
1 vol% of primary a-phase was recorded in the alloy. A primary Si
particle of around
60 mm is depicted in Figure 1(f) after leaching of the Al-phase,
from which several Si
lamellae emanate with no preferential orientation. The
interpenetrating Si networks in
the as cast condition are very sensitive to solution treatment,
disintegrating when heated
Figure 1. (a) Light Optical Micrographs (LOM) of the (a) AlSi7, (b)
AlSi12, and (d) AlSi18 alloys in the as cast condition (AC) and (c)
after spheroidization treatment (ST) in the AlSi12 (white: Al,
dark: Si); as cast self- supporting Si networks obtained after
leaching of the Al-phase from (e) AlSi7 and (f) AlSi18.
Enhanced Young’s Modulus of AlSi Alloys and Reinforced Matrices
745
at 540C. Coarse and isolated Si particles were observed after 20min
of exposure time at
540C [25]. The SFRMs present an in-plane random distribution of the
Al2O3 fibers perpendicular
to the infiltration plane (Figure 2(a)). The AlSi1.1/Al2O3/20s
matrix shows only primary a- phase since the Si content is too low
to form a eutectic. The microstructure of the compo-
sites’ matrices is similar to that of the unreinforced alloys, but
the width of the a-dendrites enclosed by the eutectic structure is
significantly smaller in AlSi7/Al2O3/20s (Figure 2(a)).
The eutectic is concentrated around fibers indicating that
solidification started at
these places. About 15 vol% primary a-phase can be observed between
the eutectic
for the AlSi12/Al2O3/20s composite (Figure 2(c)). The
AlSi18/Al2O3/20s composite
(Figure 2(d)) shows mostly a eutectic microstructure with 3 vol% of
primary Si particles,
but as well as primary a-phase dendrites. Interconnected hybrid
SiAl2O3 structures are
observed after leaching of the Al-phase. Here interconnected
networks of the eutectic Si
itself as well as of Si eutectic-plates bridging the Al2O3 fibers
are observed (Figure 2(e)).
During ST treatment, the Si plates coarsened into Si-particles,
reducing the number of
Si bridges. The Si particles sticking to the Al2O3 fibers are shown
in Figure 2(f)
(AlSi12/Al2O3/20s). Most of the Si particles become disconnected
and are lost during
leaching. The number of Si bridges is significantly reduced. The
reinforced AlSi18
Figure 2. LOM micrographs of the different short fiber reinforced
composites showing (a) the planar random distribution of the fibers
in SFRM1; higher magnification of eutectic structures in reinforced
(b) AlSi7 (c) AlSi12 in fiber plane and perpendicular planes; and
(d) AlSi18 alloys (eutectic microstructure after ST treatment in
SFRM12 perpendicular to fiber plane is presented in (c);
self-supporting SiAl2O3 networks obtained after leaching the a-Al
phase from AlSi12/Al2O3/20s in (e) as cast and (f) after ST; (g)
AlSi18/Al2O3/20s in the as cast condition showing primary Si
particles.
746 F. LASAGNI AND H. P. DEGISCHER
matrix contains eutectic Si and also primary Si particles of about
104 mm3 interconnecting
the alumina fibers (Figure 2(g)). The connectivity between the
primary Si and the fibers is
conserved even in ST condition. In AlSi7Mg/SiC/70p and
Al99.5/SiC/70p (Figure 3(a)) composites, SiC particles of
trimodal size distribution are densely packed. After the dendritic
solidification of the
primary a-phase of the AlSi7Mg matrix, the remaining eutectic
liquid (containing
12.6wt% Si) tends to solidify around the particles. The SEM
micrograph (Figure 3(b))
of AlSi7Mg/SiC/70p, where the primary a-phase has been leached off,
visualizes the Si-
bridges between the SiC particles forming a percolating SiCSi
network [14]. Of course,
such Si bridges do not exist in Al99.5/SiC/70p composite formed by
pure Al-matrix, where
the SiC particles fall apart after removal of the Al-phase. The
AlSi7/SiC/10p composite
presents a homogenous distribution of the SiC particles (Figure
3(c)) of 37 mm in dia-
meter. Particle free zones (regions in the Al-matrix which are free
of SiC particles) of
around 6 vol% are observed. The eutectic Si structure solidifies at
the SiC particles form-
ing a continuous network of SiC particles connected by eutectic Si
connected structure
(Figure 3(d)). This hybrid network is disintegrated immediately
when heated to 540C,
where Si disintegrates into isolated particles.
Figure 3. Light optical micrographs of (a) Al99.5/SiC/70p composite
showing a trimodal distribution of the SiC particles and (c)
AlSi7/SiC/10p. Porous structure obtained after leaching of the
a-phase from (b) AlSi7Mg/SiC/70p and (d) AlSi7/SiC/10p
composites.
Enhanced Young’s Modulus of AlSi Alloys and Reinforced Matrices
747
RESULTS OF YOUNG’S MODULUS DETERMINATIONS
Figure 4 and Table 4 show the experimental results for the Young’s
Modulus of the
studied matrices and composites at temperatures between 25C and
300C. The Young’s
modulus of the alloys increases with the Si content. The
hypereutectic AlSi18 alloy in the
as cast condition presents significantly higher E-values over the
entire investigated tem-
perature range compared to the other unreinforced alloys. The
Young’s modulus was
84GPa at RT and decreased to 71GPa at 300C (15% lower). The
recorded values
Y ou
ng ’s
m od
ul us
SFRM18 AC SFRM18 ST SFRM12 AC SFRM12 ST SFRM1 AC
SFRMs
Alloys
AlSi12 ST AlSi7 AC
200 250 300 350
Figure 4. Values of Young’s modulus vs. temperature for (a) the
AlSi7, 12 and 18 alloys, AlSi1-12-18/Al2O3/ 20s composites for
stresses applied in the fiber plane, and AlSi7/SiC/10p in the as
cast condition and after 540C/4 h (ST); (b) Al99.5/SiC/70p and
AlSi7Mg/SiC/70p composites.
748 F. LASAGNI AND H. P. DEGISCHER
for the hypoeutectic AlSi12 and AlSi7 in the as cast condition were
77 and 74GPa at RT, respectively. After ST treatment, a slight
reduction in the Young’s moduli to 75 and 72GPa, respectively (2%
lower), was observed for the AlSi12 and AlSi7 alloys, and 82.5
(1.7% lower with respect to AC) for AlSi18 in the ST
condition.
The stiffness of the unreinforced matrices was increased by 25% by
the addition of 20 vol% Al2O3 fibers. The Young’s modulus of
AlSi18/Al2O3/20s in the as cast condition was the highest amounting
to 106 and 91GPa at RT and 300C, respectively. In the case of
AlSi12/Al2O3/20s and AlSi1/Al2O3/20s, values of 9782GPa, and
9179GPa are observed from RT to 300C, respectively. Similar to the
unreinforced alloys, the Young’s moduli of the materials decreased
in the ST condition by 56% for SFRM18 (99GPa) and SFRM12 (92GPa) at
RT, being around 20% higher than that of the unrein- forced AlSi
alloys. On the other hand, AlSi1/Al2O3/20s exhibited the same
Young’s moduli in the as cast condition and after ST treatment,
with values of 91 and 80GPa at RT and 300C, respectively.
The addition of 10 vol% SiC particles increased the E-values of the
AlSi7 by 25%, amounting to 92GPa at 25C to 81GPa at 300C. As
observed before, the spheroidization of the Si lamellae decreased
the stiffness (by 8%) of the composite to 85 and 73GPa at RT and
300C, respectively.
DISCUSSION
For the purpose of comparison and interpretation, different elastic
models have been applied to predict the Young’s modulus of
multi-phase materials. The resulting alloy and composite moduli are
influenced by the phasemorphology, particularly the continuity of
the stiffest phase, stiffness difference of the constituents and
the volume fraction of each phase.
Table 4. Experimental Young’s modulus and theoretical predictions
(GPa).
Theoretical predictions (at RT)
(+)/() Shear
lag
AlSi7 AC 74/63 71.6/74.8 72.7 73.0/74.0 () AlSi7 ST 72/61 AlSi12 AC
77/65 74.2/80.0 76.0 76.7/78.4 () AlSi12 ST 75/63 AlSi18 AC 84/71
77.3/86.0 80.1 81.2/83.4 () AlSi18 ST 82.5/70 AlSi7/SiC/10p AC
92/81 80.5/111.4 85.2 92.7/() () AlSi7/SiC/10p ST 85/73 79/110.2
83.7 91.3/() () Al99.5/SiC/70p 220/() 169.8/335.9 215.4 260.6/() ()
AlSi7Mg/SiC/70p 242/() 175.9/336.8 220.7 264.0/() ()
AlSi1/Al2O3/20s AC 91/79 82.6/() () () 90.6 AlSi1/Al2O3/20s ST
91/79 82.6/() () () 90.6 AlSi12/Al2O3/20s AC 97/82 90.8/() () ()
97.3 AlSi12/Al2O3/20s ST 92/80 88.9/() () () 95.9 AlSi18/Al2O3/20s
AC 106/91 98.8/() () () 104.0 AlSi18/Al2O3/20s ST 99/85 () ()
103.1
Enhanced Young’s Modulus of AlSi Alloys and Reinforced Matrices
749
The appropriateness of the various models for predicting Young’s
modulus will depend on each of the above-narrated issues. The HS
lower bound is considered to be appropriate to isolated spherical
inclusions coated by a second phase. The Tuchinskii estimation
considers interpenetrating structures of the reinforcement, but
uses a simplified unit cell. The upper and lower bounds of the ROM
(Voigt and Reuss, respectively) refer to the volume fraction of the
phases without interaction and are given for comparison. The
results from the the- oretical predictions are summarized and
compared with the experimental results in Table 4.
The experimental and estimated Young’s moduli vs. Si eutectic
content for the AlSi alloys (at RT) are depicted in Figure 5. In
general, the as cast condition of the different AlSi alloys is well
represented by the Tuchinskii upper bound, where the eutectic Si
lamellae and the relatively large primary Si inclusions (in AlSi18)
form an interconnected porous structure which increases the Young’s
modulus of the alloy. The Young’s modulus of the ST samples
(containing isolated Si particles) decreases below the HS ()
estimation for particles without connectivity. The experimental
result of the AlSi12 alloy in AC falls down to the Tuchinskii lower
bound, but presenting also an enhanced Youngs modulus with respect
to the ST version.
Figure 6(b) shows the experimental results for the two 70 vol%
particle reinforced Al99.5 and AlSi7Mg matrices and their
theoretical composite predictions for the corre- sponding matrix.
The Young’s modulus of Al99.5/SiC/70p was 220GPa, while for
AlSi7Mg/SiC/70p it was 10% higher (242GPa). This difference cannot
be solely attributed to differences in matrix stiffness since the
Young’s modulus of AlSi7Mg is only 5GPa higher than that of
pure-Al. It is believed that the interconnected structure results
in the increase of the measured Young’s modulus. Supporting this is
the observation of a self-supporting interconnected SiCSi structure
after leaching of the Al-phase for the AlSi7Mg/SiC/70p composite,
where the Si lamellae connect the SiC particles (Figure 3(b)). This
was not observed for the Al99.5/SiC/70p composite in which
its
90.0
87.5
85.0
82.5
80.0
77.5
75.0
72.5
70.0
67.5
Eutectic Si (vol.%)
0 5 10 15 20 25
Figure 5. Modeled and experimental Young’s moduli at RT for pure-Al
and the different AlSi alloys.
750 F. LASAGNI AND H. P. DEGISCHER
structure is completely disintegrated during the leaching process.
Since the Si content tends
to solidify around the SiC particles in AlSi7Mg/SiC/70p (due to the
large volume content
of the reinforcing phase), a spheroidization treatment does not
reduce connectivity, and
therefore the Young’s modulus.
Y ou
ng ’s
m od
ul us
AlSi7Mg/SiC/70p Al99.5/SiC/70p
Figure 6. Experimental and estimated values of the effective
Young’s modulus in (a) AlSi7/SiC/10p in the as cast condition and
after spheroidization treatment (dash line) and (b) Al99.5/SiC/70p
and AlSi7Mg/SiC/70p composites (estimations using Al99.5 matrix are
represented in dash line).
Enhanced Young’s Modulus of AlSi Alloys and Reinforced Matrices
751
The discontinuous reinforcement phase in Al99.5/SiC/70p composite
is similar to
the HS model, which considers discontinuous spherical inclusions,
and thus it predicts
the Young’s modulus of this composite as demonstrated in Figure
6(b). In contrast,
AlSi7Mg/SiC/70p composite has the interconnected structure which
increases the
Young’s modulus near to that predicted by Tuchinskii lower bound
for interpenetrating
structures. Similarly, the Young’s modulus of the hybrid SiSiC
structure observed for
the as cast AlSi7/SiC/10p composite is well estimated by the
Tuchinskii lower bound
(Figure 6(a)). The disintegration of the network during
spheroidization treatment
decreases the stiffness of the material by 8%, falling to the HS
lower bound estimation. Figure 7 depicts the experimental values,
along with the shear lag and ROM Reuss
predictions of the Young’s modulus vs. the Si content for the
different SFRMs. Here, the
Young’s modulus is modeled for both theoretical predictions using
the experimental
matrix results of AC and ST conditions. A good agreement between
the experimental
results and the shear-lag model is observed for materials tested in
the AC condition.
From the experimental results, the Young’s modulus of AC conditions
increases by
0.4GPa/eutectic Si vol% up to the eutectic composition (12.5 vol%)
and increases
above the eutectic compositions by 1.6GPa/eutectic Si vol% for the
hypereutectic com-
positions. Note that both the shear-lag and ROM Reuss estimations
predict a higher slope
between Si 0 and 6 vol% than for 6 and 12 vol% in the hypoteutectic
range, while it is
constant in the ST samples (between Si 0 and 12 vol%). The
connectivity of the Si phase in
AC AlSi7 matrix may be responsible for this effect compared with
the almost pure Al and
ST matrices. Further investigations in materials with intermediary
Si compositions must
be carried out to confirm this observation. For the case of the
hypereutectic composition,
the addition of the primary Si particles connecting several Al2O3
fibers is considered to be
responsible for the higher slope in both AC and ST conditions.
While in SFRM12 the
110
105
100
95
90
85
80
Y ou
ng ’s
m od
ul us
Eutectic Si (vol.%)
Figure 7. Experimental and estimated values (shear lag + Reuss
model) of the Young’s modulus in AlSiX/Al2O3/20s (X¼ 1, 7*, 12,
18); *only theoretical predictions.
752 F. LASAGNI AND H. P. DEGISCHER
solution treatment decreases the Young’s moduls to the level of the
almost non-Si contain- ing SFRM, the E-value for SFRM18 in ST is
still higher than SFRM12 in AC. This may be attributed to the large
Si particles connecting the fibers in the hypereutectic composite.
Of course, the observed higher E-values with increasing Si content
is not only a consequence of connectivity, but also a result of the
addition of the stiffer Si phase (with respect to Al).
A decreasing Young’s modulus is observed in the SFRMs with Si
content >12wt% after ST treatment, dropping even below the
shear-lag estimation (with ST matrices). The shear- lag model
predicts a difference of only 1.5 and 2GPa in stiffness for SFRM12
and SFRM18, respectively, using the matrix values with
interpenetrating (AC) and isolated (ST) structures. On the other
hand, a reduction of around 5 and 7GPa was recorded experimentally
for both SFRM12 and SFRM18 composites, respectively, while for the
case of unreinforced AlSi12 and AlSi18 alloys, this difference
amounts only around 1.52GPa. The ripening of the Si lamellae
decreases the connectivity of the SiAl2O3
hybrid network in the composite materials, thus reducing the
effectiveness of the reinforce- ment and suggesting a strong
interaction between the Al2O3 fibers and the Si structure.
CONCLUSIONS
Unreinforced and reinforced AlSi alloys (containing 25 vol% or more
AlSi eutectic) present interconnected Si structures after fast
solidification (AC conditions). Hypoeutectic AlSi alloys show a
continuous Si network composed of thin interconnected Si lamellae
[25] which contribute to the stiffness of the alloys. For the case
of hypereutectic composi- tions, this network is also composed of
relatively large primary Si particles. The difference is revealed
after spheroidization of the Si phase by a solution treatment owing
to the disintegration of the Si network by decreasing slightly the
elastic modulus of the unrein- forced AlSi alloys.
The addition of Al2O3 short fibers or SiC particles to the AlSi
matrices enhances the formation of a continuous rigid structure
composed of SiAl2O3 and SiSiC networks in the as cast conditions,
which improves the Young’s modulus considerably. The effect of the
interconnected reinforcement is enhanced for composite materials,
where the disinte- gration of the SiAl2O3 and SiSiC structures by a
solution treatment decreases the Young’s modulus. On the other
hand, the Young’s modulus of AlSi1.1, AlSi1/Al2O3/20s, and
Al99.5/SiC/70p materials does not change by a ST treatment, since
the Si content is too low to form a eutectic network.
The Tuchinskii and HS lower bound predicts the effect of the
morphological changes on the materials properties. The experimental
results for the unreinforced AlSi and the PRMs with
interpenetrating structures are well estimated by the Tuchinskii
equation, while the HS lower bound is in agreement with the
experimental results for the ST or Si free PRMs (no-continuous
structures). In the case of the ST AlSi alloys, the Young’s modulus
agrees with the ROM Reuss estimation.
A good approximation of the effective Young’s modulus in the fiber
plane is obtained from the shear-lag model for the SFRMs. A
difference of only 1.5% between ST and AC conditions was predicted,
while it was more than 5% experimentally in SFRM7 and SFRM12. The
shear-lag model should be extended to the Si-bridges connecting the
fibers in the as cast condition.
Enhanced Young’s Modulus of AlSi Alloys and Reinforced Matrices
753
ACKNOWLEDGMENTS
The authors would like to thank Dr Thomas Huber for metallographic
observation and Young’s modulus estimation of the 70 vol% SiC
composites, as well as Martn Duarte and Enrique Louis of the
Alicante University for providing the AlSi7/SiC/10p samples. F.
Lasagni is grateful to funding by ARC Leichtmetallkompetenzzentrum
Ranshofen GmbH (Austria) via the Austrian
Non-Kplus-programme.
REFERENCES
1. Lasagni, F., Lasagni, A., Holzapfel, C., Mucklich, F. and
Degischer, H.P. (2006). Three Dimensional Characterization of
Unmodified and Sr-Modified Al-Si Eutectics by FIB and FIB EDX
Tomography, Advanced Engineering Materials, 8(8): 719723.
2. Lasagni, F., Degischer, H.P. and Papakyriacou, M. (2006).
Influence of Solution Treatment, Sr-Modification and Short Fiber
Reinforcement on the Eutectic Morphology of Al-Si Alloys,
Praktische Metallographie, 43(6): 271285.
3. Kelly, A. and Zweben, C. (2000). Comprehensive Composite
Materials, Vol. 3, Elsevier Science Ltd, Oxford.
4. Requena, G. and Degischer, H.P. (2004). Creep Behaviour of
Unreinforced and Short Fiber Reinforced AlSi12CuMgNi Piston Alloy,
Materials Science and Engineering: A, 420(12): 265275.
5. Schnabl, A. and Degischer, H.P. (2003). Thermal Cycling Creep of
a Short Fiber Reinforced Aluminium Piston Alloy, Zeitschrift fur
Metallkunde, 94(6): 743748.
6. Kouzeli, M. and Dunand, D.C. (2003). Effect of Reinforcement
Connectivity on the Elasto- Plastic Behavior of Aluminum Composites
Containing Sub-Micron Alumina Particles, Acta Materialia, 51(20):
61056121.
7. Peng, H.X., Fan, Z. and Evans, J.R.G. (2001). Bi-Continuous
Metal Matrix Composites, Materials Science and Engineering A,
303(12): 3745.
8. Wegner, L.D. and Gibson, L.J. (2000). The Mechanical Behaviour
of Interpenetrating Phase Composites I: Modelling, International
Journal of Mechanical Sciences, 42(5): 925942.
9. Peng, H.X., Fan, Z. and Evans, J.R.G. (2001). Bi-continuous
Metal Matrix Composites, Materials Science and Engineering A, 303:
3745.
10. Ibrahim, I.A., Mohamed, F.A. and Lavernia, E.J. (1991).
Particulate Reinforced. Metal Matrix Composites-a Review, Journal
of Materials Science, 26: 11371156.
11. Moon, R.J., Tilbrook, M., Hoffman, M. and Neubrand, A. (2005).
Al-Al2O3 Composites with Interpenetrating Network Structures:
Composite Modulus Estimation, Journal of the American Ceramic
Society, 88(3): 666674.
12. Tuchinskii, L.I. (1983). Elastic Constants of Pseudoalloys with
a Skeletal Structure, Metallurgiya, 247(7): 8592 (Translated in
Powder Metallurgy and Metal Ceramics, 85: 588595).
13. Torquato, S., Yeong, C.L.Y., Rintoul, M.D., Milius, D.L. and
Aksay, I.A. (1999). Elastic Properties and Structure of
Interpenetrating Boron Carbide/Aluminum Multiphase Composites,
Journal of the American Ceramic Society, 85(5): 12631268.
14. Huber, T., Degischer, H.P., Lefranc, G. and Schmitt, T. (2006).
Thermal Expansion Studies on Aluminium-Matrix Composites with
Different Reinforcement Architecture of SiC Particles, Composites
Science and Technology, 66(13): 22062217.
15. Elomari, S., Boukhili, R., Skibo, M.D. and Masounave, J.
(1995). Dynamic Mechanical Analysis of prestrained Al2O3/Al
Metal-Matrix Composite, Journal of Materials Science, 30(12):
30373044.
16. Puchegger, S., Loidl, D., Kromp, K. and Peterlik, H. (2003).
In: Degischer, H.P. (ed), Proceedings 14.
SymposiumVerbundwerkstoffe und Werkstoffverbunde 2003, Wiley-VCH,
Weinheim, pp. 280285.
754 F. LASAGNI AND H. P. DEGISCHER
17. Kaindl, G., Lins, W., Peterlik, H., Kromp, K., Reetz, R. and
Reetz, T. (2000). The Determination of the Elastic Moduli of
Anisotropic Ceramics and Ceramic Composites at High Temperatures by
a Novel Resonant Beam Technique, Interceram, 49(2): 92101.
18. Clyne, T.W. and Withers, P.J. (1993). An Introduction to Metal
Matrix Composites, Cambridge University Press, London, UK.
19. Hashin, Z. and Shtrikman, S. (1963). A Variational Approach to
the Theory of the Elastic Behaviour of Multiphase Materials,
Journal of Mechanics and Physics of Solids, 11: 127140.
20. Cox, H.L. (1952). The Elasticity and Strength of Paper and
Other Fibrous Materials, British Journal of Applied Physics, 3:
7379.
21. Outwater, J.O. (1956). The Mechanics of Plastics Reinforced in
Tension, Modern Plastics, 33: 5665.
22. Rosen, B.W. (1965). Mechanics of Fiber Strengthening, in Fiber
Composite Materials, American Society for Metals, Metals Park,
Ohio.
23. Dow, N.F. (1963). Study of Stresses Near Discontinuity in a
Filament Reinforced Composite Metal, GE Co., Missile and Space
Div., R635D61.
24. Dlouhy, A., Eggeler, G. and Merk, N. (1995). A Micromechanical
Model for Creep in Short Fiber Reinforced Aluminium Alloys, Acta
Metallurgica et Materialia, 43(2): 535550.
25. Lasagni, F., Lasagni, A., Holzapfel, C., Mucklich, F. and
Degischer, H.P. (2007). Three-Dimensional Characterization of
‘As-Cast’ and Solution-Treated AlSi12(Sr) Alloys by High-Resolution
FIB Tomography, Acta Materialia, 55(11): 38753882.
26. Bauccio, M. (ed.) (1994). ASM Engineered Materials Reference
Book, 2nd edn, ASM International, Materials Park, OH.
27. King, J.A. (1998). Materials Handbook for Hybrid
Microelectronics, Artech House, Nordwood, MA.